1.
Chapter 15 –Modulus of Elasticity
15. MODULUS OF ELASTICITY
The modulus of elasticity (= Young’s modulus) E is a material property, that describes its stiffness and
is therefore one of the most important properties of solid materials.
Mechanical deformation puts energy into a material. The energy is stored elastically or dissipated
plastically. The way a material stores this energy is summarized in stress-strain curves. Stress is
defined as force per unit area and strain as elongation or contraction per unit length
When a material deforms elastically, the amount of deformation likewise depends on the size of the
material, but the strain for a given stress is always the same and the two are related by Hooke´s Law
(stress is directly proportional to strain):
σ =E.ε
where
σ
is stress [ MPa ]
E
modulus of elasticity [MPa]
ε
strain [unitless or %]
From the Hook’s law the modulus of elasticity is defined as the ratio of the stress to the strain :
E=
σ
ε
[MPa]
Stress is not directly measurable. We can calculate it from different formulas for different types of the
loading (tension, flexural stress,…)
Strain is defined as the change of the length divided by the original (initial) length (see Fig.:38) :
ε=
where
∆ l l1 - l0
=
l0
l0
[unitless or
%]
∆l is change of the length [m]
l1
length after elongation [m]
l0
original (initial) length [m]
Fig.:38 Determination of the strain
F
∆l
l0
page 79
2.
Building Materials 10- Testing Methods
15.1 Graphical Determination of Modulus of Elasticity
Graphically we can define modulus of elasticity as a slope of the linear portion of the stress-strain
diagram (see Fig.:39)
Fig.:39 Graphical relationship between total strain, permanent strain and elastic strain
σ
E = tg α
σ2
2
Load
εp ……permanent strain
εel
σ1
1
…..elastic strain
Unload
part 0-1 : linear portion of stressstrain diagram
α
0
εp
α
ε1 ε2´
εtotal
εel
E = E1 =
ε2
part 1-2 :
material
σ1
ε1
plastic regime of the
E = E2 =
σ2
ε 2 − ε 2´
The line, describing unloading process of material is parallel with the linear part of stress-strain
diagram. It is evident from this, that we are able to determine modulus of elasticity even if the loading is
in the unlinear part of the stress-strain diagram. In this case we cannot calculate with whole measured
deformation (because part of the deformation is permanent), but we have to unload the material,
measure the deformation after unloading and calculate with the difference between deformation in
loaded and unloaded stage of material.
Usually we don’t know the exact shape of the stress-strain diagram of tested material before
measuring and we don’t know if the loading is in the linear or unlinear part of the stress-strain diagram.
From this reason the process of the test consists of measuring in several loaded and unloaded stages.
15.2 Determination of Modulus of Elasticity
The method that have been used to measure modulus of elasticity are following: tension (or
compression) test, bending test and natural frequency vibration test. The tension and bending test are
based on the principle of Hook’s law and they are called static methods. Measuring of the natural
frequency of vibration gives dynamic modulus of elasticity. At our laboratory lesson we will determine
static modulus of elasticity.
The static method is based on pulling or bending a sample of the material in an instrument which
measures force and measuring the changes of the length. The change of the length is usually very
small (tenths – hundredths of mm) and it is impossible to measure it by normal rules. For measuring
are used special devices – extensometers. There are several types of extensometers as mechanical or
electrical strain gauges.
page 80
3.
Chapter 15 –Modulus of Elasticity
15.2.1 Modulus of Elasticity in Tension
The test piece is mounted in the tensile testing machine which allows measurable forces to be applied.
As extensometer is used mechanical strain gauge.
Tensile stress is counted from:
σ=
where F is
A
F
A
[MPa]
applied force [N]
2
cross sectional area [m ]
Mechanical strain gauge (see Fig.:40) has two contacting point. One point is firm and the second is
movable. The distance between points is called gauge (or original) length. between points is device
which measures spacing between them. This device should be a dial where the small straight motion
of the point is transmitted into bigger rotary motion of the hand. usually there are two hands – big hand
showing divisions on main scale (centesimal or millesimal) and small hand, showing whole millimetres
on auxiliary scale.
The change of the length is count as difference between gauge reading in the state of loading and
gauge reading in unloaded state.
Fig.:40 Mechanical strain gauge
firm point
gauge (original) length l0
test piece
dial
movable point
15.2.2 Modulus of Elasticity in Flexural Stress
The test piece is supported at either end and load (in a form of weights) is applied in the middle
between the supports . As extensometer is used electrical resistance gauge.
Flexural stress is counted from:
σ=
M
W
page 81
4.
Building Materials 10- Testing Methods
where M is
W
2
bending moment [ N. mm ]
3
section modulus [ mm ]
Some basic examples of loading and appropriate formulas for bending moment and section modulus
are given in tab.3 ( in chapter 3 ).
The principal of electrical resistance gauge is based on the fact that a change in electrical resistance is
proportional to the strain, i.e. ∆R/R is function of ε.
Electrical resistance gauge consists of a thin wire grid, fixed on foil (usually paper). The gauge is
bonded to the strained surface of measured material by a thin layer of a special glue. (see Fig.:41).
Fig.:41 Electrical resistance gauge
B
C
D
A
B
C
tested material
wire grid
connected leads
D
E
basic foil
glue layer
The change of resistance is proportional to strain according formula:
where l is
1
Λl
ΛR
=
×
l
K
R
length of the wire
R
electrical resistance
K
gauge factor
The ideal strain gauge would change resistance only due to the deformations of the surface to which
the gauge is attached. However, in real applications, temperature, material properties, the adhesive
affect the detected resistance.
Internal influences (as materials properties of wire, type of used glue, size of the wire and the shape of
the wire grid) are considered in gauge factor K.
The external influences (the changes of the temperature and moisture) have to be considered in a type
of measuring circuit.
In order to measure strain with a bonded resistance strain gauge, it must be connected to an electric
circuit that is capable of measuring the small changes in resistance corresponding to strain. Usually
the Wheatstone bridge is used, this circuit is also well suited for temperature compensation.
Wheatstone bridge is a four arm, four-terminal resistance –measuring network.( see Fig.:42 )
page 82
5.
Chapter 15 –Modulus of Elasticity
Fig.:42 Scheme of Wheatstone bridge
C
R1
If the formula:
R2
B
D
Vout
R3
Vin
R1 R3
is valid and voltage
=
R 2 R4
Vin is applied between points A and C, then
the output between B and D will show no
potential difference = the Wheatstone bridge
is balanced (the galvanometer between B
and D shows zero).
If R1 is changed to some value which does
not equal R2, R3, R4, the bridge will become
unbalanced and a voltage will exist at the
output terminals.
R4
A
Measuring scheme by apparatus TSA is given in Fig.:43. Resistance R1 is a measuring gauge, bonded
on tested material in the place of measured deformations. Resistance R2 is compensating gauge. It is
the same type of gauge as R1, but bonded on non-loaded piece of material. It is used for temperature
compensation, but not for strain measurement. The resistance changes due the temperature will have
the same value for R1 and R2. This changes will cancel, because in the formula for balanced bridge
resistances R1 and R2 are in ratio. Unbalance of the bridge will than caused only changes of R1 from
deformations.
Fig.:43 Measuring of modulus of elasticity by the electrical resistant gauge
Fi
R1
measuring gauge
R3
0.057
compensating
gauge
R2
R4
variable resistance for
balancing of the bridge
page 83
6.
Building Materials 10- Testing Methods
Resistances R3 and R4 are the components of tensometric apparatus. R3 is adjustable and serves for
nullification of gauge factor. Value of R3 can be set up in advance. Resistance R4 is a potentiometer
(variable resistance), by it the bridge can be balanced again. The dial of the potentiometer has scale
division straight in values of the strain.
15.2.3 Determining of the Basic Strain at Basic Loading
From several reasons it is impossible to measure stress and strain in the low loading range (close to
zero loading). Mechanical and electrical machines have lost motions (motion is initiated, but you don’t
see any results for some time), or there is a risk of the specimen’s falling-out from jaws.
If we determine initial modulus of elasticity (i.e. from zero loading to the appropriate loading), we
cannot measure deformations straight from zero loading, we begin to measure from some basic
loading F0. We are able to determine basic part of deformations ε0 (from zero to F1) from linear part of
the stress-strain diagram (see Fig.:44 ) by calculation or graphically from similarity of triangles.
Fig.:44 Extrapolation of stress-strain curve in the low loading range
σ
σi
σ´
σ0 …
σ1 …
1
σ0
0
ε1 ´
ε i´
strain at loading F 1
ε0
σ1
stress at loading F 1
ε 1´ …
i
ε1 ´
basic stress (at F0 )
basic strain (from 0
to F 1 )
…
From sim ilarity of triangles:
ε´
ε 0 = ε ′1 ×
ε
ε0
ε1
εi
Total strain at loading Fi is than :
εi = ε0 + ε′
i
where εi is
total strain from zero to appropriate loading Fi
εi ´
ε0
page 84
strain from F1 to appropriate loading Fi
basic strain from zero to F1
F0
F1 - F0
7.
Chapter 15 –Modulus of Elasticity
Tab.:36 Value of modulus of elasticity for some materials
Material
Modulus of elasticity
aluminium and its alloys
65 - 73
ceramics
8 - 12
concrete
15 - 40
copper
125
diamond
1000
lightweight concrete
0,8 - 2
low alloy steels
200 - 210
polystyrene
3,2 - 3,5
silica glass
60 - 90
wood
[GPa]
11-16
Vocabulary
balanced Wheatstone bridge
Wheatstoneův můstek v rovnováze
compensating gauge
kompenzační tenzometr
dial strain gauge
číselníkový úchylkoměr
elastic strain
pružná (elastická) deformace
electrical resistance strain gauge
elektrický odporový tenzometr
gauge factor
konstanta tenzometru
initial modulus of elasticity
počáteční modul pružnosti
lost motion
mrtvý chod
measuring gauge
měřící tenzometr
mechanical strain gauge
mechanický tenzometr
permanent strain
trvalá (plastická) deformace
slope
směrnice
stiffness
tuhost
strain
deformace
strain gauge
tenzometr
stress
napětí
stress-strain diagram
pracovní diagram
total strain
celková deformace
Wheatstone bridge
Wheatstoneův můstek
page 85
8.
Building Materials 10- Testing Methods
Fig.:45 Example of calculation of modulus of elasticity
page 86
Be the first to comment